Download presentation

Presentation is loading. Please wait.

Published byTess Burkley Modified over 2 years ago

1
**Acero 2000 PHYSICAL METALLURGY AND THERMAL PROCESSING OF STEEL**

Ernesto Gutierrez-Miravete Rensselaer at Hartford Monterrey, Mexico, Julio, 2000

2
**Course Outline 1.- Physical Metallurgy of Steel**

2.- Phase Transformations in Steel 3.- Solidification of Steel 4.- Heat Treatment of Steel 5.- Welding and Surface Treatment of Steel 6.- Supplementary Reading

3
**1.- Physical Metallurgy of Steel**

1.1.- Iron 1.2.- Iron-Carbon Alloys 1.3.- Steels

4
1.1.- Iron Thermodynamic Properties Phases Crystal Structures

5
**1.2.- Iron-Carbon Alloys Crystal Structures Phases and Microstructures**

Thermodynamic Properties Phase Diagram

6
**1.3.- Steels Alloying Elements Phase Diagrams Thermodynamic Properties**

Structural Effects Diffusion Real Surfaces

7
**Iron, Iron Alloys and Fe-C system**

Medium of first transition series: Ar3d64s2 Earth Crust contains ~ 4% Fe Tf =1540 C ; Th ~ 750 C Useful Phase Transformations (bcc-fcc) Ferromagnetic below 768 C

8
**Iron, Iron Alloys and Fe-C system (contd)**

Interstitials: H, B, C, N, O Substitutionals: Mostly transition series left, right and below of Fe Fe-C system is the basis of steel metallurgy

9
**Phases and Phase Diagrams**

Equilibrium Phases Ferrite (: T < 906, : 1401 < T <1540 C) Austenite (: 906 C < T < 1401 C) Liquid (l: T > 1540 C) Carbide, Nitride, Oxide Compounds Phase Diagrams Graphic display of stable phases as function of temperature.

10
**Crystalline Structures, Microconstituents and Microstructures**

Equilibrium Crystal Stuctures Ferrite (Body Centered Cubic; BCC) Austenite (Face Centered Cubic; FCC) Carbides, Nitrides, Oxides (Complex)

11
**Crystalline Structures, Microconstituents and Microstructures (contd)**

Equilibrium Microconstituents Ferrite Austenite Pearlite (Ferrite-Carbide Micro-Composite)

12
**Crystalline Structures, Microconstituents and Microstructures (contd)**

Equilibrium Microstructures Ferrite (Grains, Allotriomorphs, Widmanstatten Side-Plates) Austenite (Grains - Twinned) Pearlite (Ferrite-Carbide Colonies)

13
**Crystal Defects Vacancies Dislocations Stacking Faults**

Nv = C exp(- U/kT) Dislocations -Fe (a/2)<111> -Fe (a/2)<110> Stacking Faults -Fe High SFE -Fe Low SFE ( Twinning)

14
**Crystal Defects (contd)**

Grain Boundaries Low Angle High Angle Interstitial and Substitutional Atoms Interphase Interfaces Coherent Semi-coherent Incoherent

15
**Crystal Defects (contd)**

Gibbs-Thompson Equation ln (c(r)/c) = 2 V/r R T Surfaces Crystalline arrangement Surface strain Chemical layering

16
**Multilayer Structure of Real Surfaces**

Steel Decarburized steel Steel-Oxide transition zone Wustite layer Magnetite layer Haematite layer

17
**Effects of Alloying Elements**

Physico-chemical properties Mechanical properties Magnetic properties Corrosion resistant properties

18
**Alloying Elements Expanded -field Contracted -field**

Open (Ni, Co, Mn, Ru, Rh, Os, Ir, Pt) Compunds (C, N, Cu, Zn, Au) Contracted -field Closed (Si, Al, Be, P, Ti, V, Mo, Cr) Compounds (Ta, Nb, Zr)

19
**2.- Phase Transformations in Steel**

2.1.- Temperature-Time Charts 2.2.- Mathematical Modeling of Thermal Processing of Steel 2.3.- Phase Transformations during Cooling 2.4.- Phase Transformations during Heating 2.5.- Research Techniques

20
**2.1.- Temperature-time Charts**

Casting and Cooling of Liquid Steel Heat Treating Thermomechanical Processing

21
**2.2.- Mathematical Modeling of Thermal Processing of Steel**

Diffusion Heat Transfer Fluid and Solid Mechanics Electromagnetism Microstructural Evolution

22
**2.3.- Phase Transformations during Cooling**

Solidification Pearlite Formation Ferrite Formation Cementite Formation Bainite Formation Martensite Formation

23
**2.4.- Phase Transformations during Heating**

Recrystallization Austenitization Tempering Melting

24
**2.5.- Research Techniques Metallography Microscopy Crystallography**

Mechanical Testing Thermometry Mathematical Modeling

25
**Phase Transformations**

Continuum Rate Equations: Convection, Difusion of Mass, Energy and Electromagnetic Fields, Kinetics Phase Transformation Kinetics Additional Microconstituents Isothermal and Continuous Cooling Transformation Diagrams

26
**Continuum Rate Equations**

Conservation of Mass (Eqn. of Continuity) Conservation of Momentum (Eqn. of Motion) Conditions of Compatibility Conservation of Energy (Energy Eqn.)

27
**Continuum Rate Equations (contd)**

Conservation of Species (Diffusion Eqn. and/or Convection/Diffusion Eqn.) Maxwell’s Equations Constitutive Equations Boundary Conditions Arrhenius Rate Equation r = A exp(- E/kT)

28
**Phase Transformation Kinetics**

Diffusive Nucleation-Growth Transformations f = (4/3) Sot I G3 (t - )3 d f = 1 - exp(- a tb) Displacive Transformations (T < Ms) f = max {1 - exp( - K0 [Ms - T])} Diffusive-Displacive Transformations

29
**Phase Transformation Kinetics (contd)**

Grain Growth ( d = grain diameter) d/t = K1 exp(-Q/k T) d (1 - 1/n) Precipitate Growth/Dissolution (diffusion controlled) ( r = precipitate radius) r/t = {2 D V c / r R T}{ 1/rm - 1/r}

30
**Phase Transformation Kinetics (contd)**

Precipitate Growth/Dissolution (interface controlled) r/t = {2 K2 V c/ R T}{ 1/rm - 1/r} Analytical solution (dilute solution) r2 - ro2 = 2 a C D t where C = (ci - ce)/(cp-ce) << 1 and a = 1 + ro/( D t) 1/2

31
**Phase Transformation Kinetics (contd)**

Solute balance at a steady state moving solid-liquid interface - D (c/x) = V (cL* - cS*) = V co (1/k - 1) i.e. c(x) = co + co (1/k - 1) exp[ - V x/D] Solid-liquid interface stability condition G < m Gc = m V (cL* - cS*)/ D

32
**Phase Transformation Kinetics (contd)**

Dendritic growth (primary spacing) 1 = K3 /V1/4 G 1/2 Dendritic growth (secondary spacing) 2 = K4 ts1/3 Eutectic growth (interlamellar spacing) e = K5 V1/2

33
**Non-Equilibrium Microconstituents**

Martensite Body Centered Tetragonal; BCT C-supersaturated Ferrite Laths, Plates, Needles Bainite BCC-BCT Ferrite-Carbide Micro-Composite Laths, Plates

34
**Isothermal Transformation Diagrams**

path 1 path 2 path 3 t

35
**Continuous Cooling Transformation Diagrams**

path 1 path 3 path 2 t

36
**Properties of Individual Microconstituents in Steel**

High-purity Ferrite (single crystal) Theoretical yield shear stress ~ 2000 MPa Actual yield shear stress ~ 10 MPa High-purity Ferrite (polycrystal) Theoretical yield shear stress ~ 6000 MPa Actual yield shear stress ~ MPa Grain size dependence = o +K /d1/2

37
**Properties of Individual Microconstituents in Steel (contd)**

Pearlite Yield strength MPa Tensile strength MPa Bainite Yield strength MPa Tensile strength MPa Martensite Yield strength MPa

38
**Steel as a Composite Material**

Rule of Mixtures = a fa + b fb Empirical relations (low C steel) = 15.4 { (%Mn) + 5.4 (%Si) (%pearlite) + 0.5/d 1/2}

39
**Steel as a Composite Material (contd)**

Empirical relations (eutectoid steel) = /d1/2 where d = interlamellar spacing (mm)

40
**Strengthening Mechanisms in Steel**

Solid Solution Strengthening Dispersion Hardening Dislocation Strengthening Grain Boundary Strenghening

41
**Thermal Processing Techniques and Thermometry**

Heating and Cooling Induction and Resistance Heaters High Energy Density Beams Molds Quenching Baths Thermometry and Dilatometry Temperature Measurement Volume Measurement

42
**Diffractometry/Quantitative Metallography/Image Analysis**

X-Rays Electrons Neutrons Microscopy Optical Electron Field Ion

43
**Diffractometry/ Quantitative Metallography/Image Analysis (contd)**

Image acquisition Digital processing Thresholding operations Mathematical morphology operations Measurements

44
Mechanical Testing Hardness test Tensile test Creep test Fracture test Fatigue test

45
**Mathematical Modeling and Computer Simulation**

Hardware PC Workstations Supercomputers Software Custom -made Research Commercial

46
**Reading Verhoeven et al, JOM, Sept 1998**

Sundman & Agren, MRS Bull, Apr 1999

47
**3.- Thermal Processing of Liquid Steel**

3.1.- Liquid-Solid Transformations 3.2.- Microstructure Formation during Solidification 3.3.- Macrostructure Formation during Solidification 3.4.-Mathematical Modeling of Steel Solidification

48
**3.1.- Liquid-Solid Transformations**

Melting and Solidification of Pure Iron Solidification of Liquid Steel to Primary Delta-Ferrite Solidification of Liquid Steel to Primary Austenite Melting of Alloy Additions in Liquid Steel

49
**3.2.- Microstructure Formation during Solidification**

Nucleation of Crystals Dendritic Growth The Peritectic Transformation during Steel Solidification Microsegregation

50
**3.3.- Macrostructure Formation during Solidification**

Formation and Evolution of the Mushy Zone during Solidification of Steel Solute Transport and Settling/Floating of Crystals in the Melt Macrosegregation Contraction during Solidification Stresses from Solidification

51
**3.4.-Mathematical Modeling of Steel Solidification**

Heat Transfer Solute Transport Microstructural Evolution Stress Generation

52
**Reading Vanaparthy & Srinivasan, Mod. & Sim. in MSE, Vol. 6, 1998**

Schwerdtfeger at al, Met & Matls Trans B, Oct 1998

53
**4.- Heat Treating of Steel**

4.1.- Hardenability 4.2.- Austenitizing 4.3.- Annealing 4.4.- Quenching 4.5.- Tempering 4.6.- Mathematical Modeling

54
**4.1.- Hardenability Concept of Hardenability**

Physical Foundation of Hardenability Measurement of Hardenability Influence of Hardenability on Structure and Properties

55
4.2.- Austenitizing Nucleation and Growth of Austenite during Austenitization Dissolution of Carbides during Austenitization Austenite Grain Growth during Austenitization

56
**4.3.- Annealing Phase Transformations during Isothermal Holding**

Nucleation and Growth of Ferrite Nucleation and Growth of Pearlite Nucleation and Growth of Cementite

57
**4.4.- Quenching Phase Transformations during Continuous Cooling**

Nucleation and Growth of Bainite The Martensitic Transformation Formation of Composite Microstructures containing Multiple Microconstituents Dimensional Changes

58
**4.5.- Tempering Precipitation and Growth of Carbides during Heating**

Transformation of Retained Austenite during Heating Change of Physical Properties during Tempering Dimensional Changes

59
**4.6.- Mathematical Modeling of Heat Treatment of Steel**

Heat Transfer Solute Transport Microstructure Evolution Stress Generation

60
**Reading Homberg, Acta Mater. Vol. 44, 1996**

Inoue & Arimoto, J. Matls Eng. & Perf., Feb 1997 Archambault et al, J. Matls Eng. & Perf., Feb 1997

61
**5.- Welding and Surface Treatment of Steel**

5.1.- Welding of Steel 5.2.- Case Hardening of Steel 5.3.- Surface Hardening by Rapid Heating and Cooling

62
**5.1.- Welding of Steel Welding Process**

Weld Microstructure and Properties Mathematical Modeling

63
**5.2.- Case Hardening of Steel**

Case Hardening Processes Solute Diffusion from the Surface of Steel Decarburization of Steel on Heating Nitriding Mathematical Modeling

64
**5.3.- Surface Hardening by Rapid Heating and Cooling**

Diffusion of Time-Varying Electromagnetic Fields into Steel Surface Heating by Eddy Currents Surface Heating by Focused Beams Phase Transformations during Rapid Surface Heating Mathematical Modeling

65
**Reading Mundra et al, Weld. J. WRS, Apr 1997 Bhadeshia, 1999**

Mittemeijer & Somers, Surf. Eng, Vol. 13, 1997 Fuhrmann & Homberg, 1999

Similar presentations

© 2017 SlidePlayer.com Inc.

All rights reserved.

Ads by Google